International Journal of Photoenergy
Volume 2019 (2019), Article ID 6292036, 5 pages
https://doi.org/10.1155/2019/6292036

Research Article

Optimization of Helium Inflating on Heat Dissipation and Luminescence Properties of the A60 LED Filament Lamps

Yizhan Chen, Qingguang Zeng, Lite Zhao, Yuanxing Li, Guangyao Huang, and Bingqian Li

School of Applied Physics and Materials, Wuyi University, Jiangmen, Guangdong, China

Correspondence should be addressed to Yizhan Chen; yizhanchen@126.com

Received 15 September 2018; Revised 12 January 2019; Accepted 14 February 2019; Published 2 April 2019

Academic Editor: Alberto Álvarez-Gallegos

Copyright © 2019 Yizhan Chen et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

LED filament lamp has the characteristics of nearly 360° lighting angle, high brightness, and low energy consumption, turning it gradually into the best substitute for traditional incandescent lamps. At present, due to the limitations of heat dissipation, the development of high-power LED filament lamp is restricted. Helium is a rare gas with small density and high heat transfer coefficient. It can be used as a cooling and protective gas for LED filament lamp. In this paper, we investigated the effects of helium on the heat dissipation and luminescence performance of the A60 LED filament lamps by detecting the changes of junction temperature, color temperature, and luminous flux of different ratios helium inflating in the different power A60 LED filament lamps. Through the experiment, we found the most cost-effective ratio of helium gas in the A60 LED filament lamps without improving the lamp size and the filament diameter.

1. Introduction

The LED filament lamp has both the appearance of the traditional incandescent lamp and the higher photoelectric conversion of LED lamp. In 2008, Ushio Lighting introduced the first LED filament lamp [1]. Panasonic described a flat arrangement with modules similar to filaments in 2014 [2]. Unfortunately, the products did not gain widespread market acceptance due to the poor thermal dissipation and luminous flux. This paper investigates the heat dissipation to increase the luminescence of LED filament lamp. The LED filament lamp was usually made up of chips, transparent substrate, and phosphors [3]. According to the development of substrate materials, LED filament lamps have undergone three generations from transparent ceramics, quartz glass to sapphire [4, 5].

Although the LED filament lamp has the basic structure similar to the traditional incandescent lamp, its luminous structure is essentially different from the incandescent lamp. The incandescent lamp relied on the tungsten filament to emit visible light at high temperature, while the LED filament lamp relied on filaments of the LED. However, because the phosphor completely wrapped around the filament, the heat dissipation effect of the filament was limited [6], which was also the main reason to restrict the high power of LED filament lamp [7].

Besides the lamp size, the filament phosphor diameter, and ionic wind [8, 9], this paper mainly explored the application of helium inflating to enhance the heat dissipation effect of LED filament lamp. As the helium is one of the inert gases, with its low density and high thermal conductivity, it was very suitable to be used to extract heat from the LED filaments [10, 11]. In this paper, the influence of helium on the heat dissipation and luminous performance of LED filament lamps was explored by detecting the change of the temperature and luminous flux of different helium ratios at the A60 LED filament lamps with different power.

2. Experimental and Theoretical Details

2.1. Thermal Conductivity of Helium

This paper explored the heat dissipation and luminescent properties of LED filament lamps filled with helium. Helium is a colorless and tasteless inert gas. Under normal pressure and temperature, the density of helium is 0.178 g/L. The helium molecule is very small and is just placed behind the hydrogen with the smallest density. As shown in Table 1, the thermal conductivity of helium is 0.144 W/(m·°C) which is a little smaller than the thermal conductivity of hydrogen 0.163 W/(m·°C). As an inert protective gas, helium does not react with the material in the LED filament lamp. In Table 1, the thermal conductivity of helium is higher than argon, neon, oxygen, nitrogen, and air. This was the reason why helium was chosen for heat dissipation and gas protection.

Table 1: Thermal conductivity of several common gases.

Gas
Hydrogen
Helium
Argon
Neon
Oxygen
Nitrogen
Air

Thermal conductivity (W/(m·°C))
0.163
0.144
0.018
0.049
0.024
0.023
0.023

2.2. Convective Heat Dissipation Mechanism of the A60 LED Filament Lamp

The A60 LED filament lamp was the spherical shell with a maximum diameter of 60 mm, as shown in Figure 1. In our experiment, the power values of the A60 LED filament lamps were 4 W, 7 W, and 8 W. The chips were spot welded in series on the holder of filament to form the LED filament. The holders of the filament and LED filament are shown in Figure 2. These four LED filaments were in series to form the A60 LED filament lamp. A linear drive was provided in the lamp holder to support a stable current input for the LED lamp. The driving currents of 4 W, 7 W, and 8 W in the A60 LED filament lamps were 13.5 mA, 22 mA, and 25 mA, respectively.

(a)

(b)

Figure 1: (a) The A60 LED filament lamp and (b) its structure parameters.

Figure 2: (a) Holder of the filament and (b) LED filament in the A60 lamp.

In the whole lamp, the heat is transferred from the LED filament to the helium when the helium is passing through the LED lamp in the high-temperature work. The density of the heating helium is smaller than the helium at the low temperature, so the expansion rises. And the heat is transferred to the glass shell from the filament, and then the next cycle starts. In the whole process, gas heat conduction followed Fourier law [12]. This phenomenon is affected by the natural factors of the fluid itself. When applied to fluid cooling, convection calculation is shown as follows:

Among them, is the convection heat dissipation (the unit is ), and is the thermal conductivity (the unit is W/m·°C). is an effective heat transfer area. The temperature difference between the heat transfer surface and the fluid is . The Fourier law can be applied to the convection heat transfer process. In the process of heat convection in the lamp, according to equation (1), the thermal conductivity is the key factor affecting convective heat transfer under the condition of the same temperature difference and the same area.

2.3. The Effect of Chip Junction Temperature on the Performance of LED

The relationship between the main wavelength of LED filament lamp and the junction temperature of the chip is shown as follows:

In equation (2), and are the main wavelengths of the emitted light at and , respectively. is the temperature difference, that is to say the main wavelength of the chip changed correspondingly with the temperature difference, thus changing the spectral composition of the chip [13]. The increase of the junction temperature also affected the color temperature of the LED filament lamp, making the color temperature drift. The lifetime of LED chip increased exponentially with the decrease of the junction temperature. When the temperature of the chip rises from 40°C to 50°C, the life span of the chip could be shortened from 42,000 hours to 18,000 hours [14]. In this paper, through the influence of helium on the heat dissipation, luminescence performance and color temperature of the A60 LED filament lamps were explored by detecting the change of the junction temperature and luminous flux in the A60 LED filament lamps with different powers.

2.4. Testing Measurements

The instrument LEDT300/H was specially designed and developed for measuring the junction temperature of LED filament lamps. The main test method was to put the test lamp in the chamber of the LEDT300B/H and then connected the thermocouple with the current input line of the lamp to test the junction temperature. That was because the junction and the current input line connected directly, the temperatures between them were the same. When the lamp was working in the normal working voltage range, the exact value of the working voltage was obtained when it reached the stable state, and the junction temperature of the lamp in the stable operation was obtained by combining the value of the voltage temperature coefficient.

The spectrum integration sphere PMS-80 was mainly used to test the photoelectric parameters of the LED filament lamps. The working way of the integral ball was to place the test light source or lamp in the center of the integral ball. After applying the working voltage, the light was reflected multiple times on the inner wall of the integrating sphere and finally concentrated on the window hole. The external connecting device of the integrating sphere concentrated the light at the window hole and finally calculated the photoelectric parameters of the test light source or the lamp, which included the parameters of luminous flux and color temperature.

3. Results and Discussion

The positive chip mode was used in the A60 LED filament lamps to meet the process stability in this experiment. The transparent ceramic substrate was used to improve their performance price ratio in this lamp. The A60 LED filament met the European state standard. The A60 LED filament with a power of 4 W had a size of , with 24 LED chips in series. The LED filaments with the powers of 7 W and 8 W both had the sizes of , containing 25 LED chips in series inside. The difference between them was the power of the internal LED chips. The following figures are about the junction temperature and luminous properties of the A60 LED filament lamps (powers of 4 W, 7 W, and 8 W) under different helium inflating quantities (50%, 60%, 70%, 80%, and 90%) with the different pressures ranged from 0.5 Pa to 0.9 Pa. The junction temperature, luminous flux, and color temperature data diagram were tested at room temperature of 25°C.

3.1. Influence of Different Helium Inflating Ratios on the Junction Temperature of the A60 LED Filament Lamps

It can be seen from Figure 3 that with the increase of helium gas inflating, the junction temperature of all the A60 LED filament lamps decreased. For the 8 W power LED filament lamp, the lowest helium inflating ratio of 50% got the highest junction temperature of 113.5°C. In the same inflated helium proportion, the 4 W filament lamp had the lowest junction temperature. This was because the power value of 4 W was lower, the working current was smaller, and the heat also reduced accordingly. Compared with the A60 LED filament lamp with different power charge, the higher inflating ratio was conducive to the heat dissipation of the filament and the junction temperature.

Figure 3: Junction temperatures of the A60 LED filament lamps (4 W, 7 W, and 8 W) with different helium inflating ratios.

In Table 2, the A60 LED filament lamps were driven under the power 4 W and the voltage 270 V. Compared with the LED filament lamps of 4 W power, the A60 LED filament powers and junction temperatures of 7 W and 8 W obviously reduced. Because the substrate size of the 7 W and 8 W power filaments was much larger than the 4 W power filament, the heat dissipation was faster. The 7 W and 8 W power filaments had the length of 50 mm, while the 4 W power filament had only 38 mm. Apart from that, the heat exchange area of 4 W power filament was smaller. Therefore, both the helium gas inflating and the size of filament influenced the heat dissipation.

Table 2: A60 LED filament lamp junction temperatures and filament lamps under 4 W-driven power.

Lamp type/W
4
7
8

Junction temperature/°C
92.40
79.9
69.12

Filament power/W
3.807
3.55
3.445

3.2. Influence of Different Helium Inflating Ratios on Luminous Flux of the A60 LED Filament Lamps

Figure 4 is the luminous flux data of the three different power A60 LED filament lamps under different ratios of helium inflating. For the same power level, the luminous flux increases as the ratio of helium inflating increases. It can be explained by the fact that the junction temperature decreases with the helium inflating ratio.

Figure 4: Luminous flux changed with different helium inflating ratios in the A60 LED filament lamp.

In this experiment, we found that with 80% helium inflating, the luminous flux of the A60 LED filament lamps were 480 lm, 815 lm, and 1070 lm for the power values of 4 W, 7 W, and 8 W, respectively. These values were higher than the nominal luminous flux of the commercial A60 LED filament lamps of 470 lm, 806 lm, and 1055 lm also for the power values of 4 W, 7 W, and 8 W, respectively. At the value of 80% helium gas inflating, these series of the A60 LED filament lamps can maintain the nominal luminous flux value requirement, saving more energy than the lamp with helium ratio of 90% and improving the performance price ratio.

3.3. Influence of Different Helium Inflating Ratios on the Color Temperature of the A60 LED Filament Lamps

Figure 5 shows the color temperature of the three power A60 LED filament lamps at different helium inflating ratios. The inflating ratio affected the junction temperature of the filament, and the junction temperature affected the color temperature change. From the data, it can be seen that the color temperature of the A60 LED filament lamp of every power decreased with the increase of the inflatable ratio, which was in accordance with equation (2) that the temperature of the filament affected the color temperature of the filament. Of course, the main factor determining the color temperature of LED filament was the ratio of blue and yellow phosphor.

Figure 5: Color temperature changed in the A60 LED filament lamps of different helium inflating ratios.

4. Conclusions

From the experimental analysis, it was found that the higher helium inflating ratio had a significant effect on the heat dissipation and luminous properties of the A60 LED filament lamps. In the case of low helium inflating ratios, the increase of helium volume can brought obvious performance improvement. The direction for the improvement of LED filament lamp is to develop high-power LED filament lamps. The greater power value means that the filament needs to carry higher current, leading to higher junction temperature. The high junction temperature had a heavy influence on the luminous flux, color temperature, and life of the A60 LED filament lamp. Therefore, the thermal analysis of LED was very important for judging the feasibility of LED filament lamps. A good balance between luminous flux and helium inflating volume helped enterprises to reduce the cost of LED filament lamps and improve their performance. In our research, we found that with 80% of helium inflating without changing the size of the lamp and filament, the A60 LED filament lamp can maintain the nominal luminous flux value requirement. Consequently, it can reduce more costs than a lamp with helium ratio of 90% and improves the performance and market competitiveness of the A60 LED filament lamp with different power values.

Data Availability

The data used to support the findings of this study are included within the article.

Conflicts of Interest

The authors declare that they have no conflicts of interest.

Acknowledgments

The authors greatly appreciate the support of the Key Laboratory of Optoelectronic Materials and Applications in Guangdong Higher Education (No. 2017KSYS011), the Key Platform Construction Center Project in Guangdong Department of Education (No. GCZX-A1411), and the Youth Fund Project in Wuyi University (No. 2015zk13). The authors appreciatively acknowledge discussions with and manuscript editing by Prof. Norbert Willenbacher and Ph.D. candidate Bruna R. Maciel at Karlsruhe Institute of Technology in Germany.

References

K. Hakata and T. Matsuoka, “Light-emitting device and lighting apparatus incorporating same,” US Patent 8400051B2, 2009.

T. Nobuyoshi, M. Tsugihiro, N. Hideo, M. Masahiro, and U. Takaari, “Light bulb shaped lamp and lighting apparatus,” US Patent 8858027B2, 2013.

D. Chen, H. Zheng, Z. Huang et al., “Light-emitting diode-based illumination system for in vitro photodynamic therapy,” International Journal of Photoenergy, vol. 2012, Article ID 920671, 6 pages, 2012.

C. G. Yan, The Key Technology of LED Filament Design, LED Good Products Magazine, 2014, fifty-third stage.

M. W. Jeong, S. W. Jeon, S. H. Lee, and Y. Kim, “Effective heat dissipation and geometric optimization in an LED module with aluminum nitride (AlN) insulation plate,” Applied Thermal Engineering, vol. 76, pp. 212–219, 2015.

M. Arik, C. A. Becker, S. E. Weaver, and J. Petroski, “Thermal management of LEDs: package to system,” in Third International Conference on Solid State Lighting, vol. 5187 of Proceedings of SPIE, pp. 64–75, Bellingham, WA, USA, 2004.

X. Luo, R. Hu, S. Liu, and K. Wang, “Heat and fluid flow in high-power LED packaging and applications,” Progress in Energy and Combustion Science, vol. 56, pp. 1–32, 2016.

J. Liu, C. Xu, H. Zheng, and S. Liu, “Numerical analysis and optimization of thermal performance of LED filament light bulb,” in 2017 IEEE 67th Electronic Components and Technology Conference (ECTC), pp. 2243–2248, Orlando, FL, USA, 2017.

C. Xu, Z. Zhang, J. Chu et al., “Thermal dissipation enhancement of LED filament bulb by ionic wind,” in 2016 17th International Conference on Electronic Packaging Technology (ICEPT), pp. 1212–1215, Wuhan, China, 2016.

W. Feng, B. Feng, F. Zhao, B. Shieh, and R. Lee, “Simulation and optimization on thermal performance of LED filament light bulb,” in 2015 12th China International Forum on Solid State Lighting (SSLCHINA), pp. 88–92, Shenzhen, China, 2015.

C. Sciascia, A. Corazza, G. Santella, H. Sato, and S. Giorgi, “Beneficial effect of optimized gas filling in gas cooled LED bulbs,” Journal of Science and Technology in Lighting, vol. 41, pp. 96–100, 2018.

S. Lepri, R. Livi, and A. Politi, “Thermal conduction in classical low-dimensional lattices,” Physics Reports, vol. 377, no. 1, pp. 1–80, 2003.

C. Qian, “Thermal management of high-power white LED package,” in 2007 8th International Conference on Electronic Packaging Technology, pp. 1–5, Shanghai, China, 2007.

N. Narendran and Y. Gu, “Life of LED-based white light sources,” Journal of Display Technology, vol. 1, no. 1, pp. 167–171, 2005.